Raman Spectroscopy and Time-Resolved Photoluminescence of BN and BxCyNz Nanotubes
2004 Vol. 4, No. 4 647-650
J. Wu,† Wei-Qiang Han,†,‡,§ W. Walukiewicz,*,† J. W. Ager III,† W. Shan,† E. E. Haller,†,| and A. Zettl†,‡,§ Materials Sciences DiVision, Lawrence Berkeley National Laboratory, Berkeley, California 94720, Department of Physics, UniVersity of California, Berkeley, California 94720, Molecular Foundry, Lawrence Berkeley National Laboratory, Berkeley, California 94720, and Department of Materials Science and Engineering, UniVersity of California, Berkeley, California 94720 Received January 22, 2004; Revised Manuscript Received March 3, 2004
ABSTRACT We report Raman and time-resolved photoluminescence spectroscopic studies of multiwalled BN and BxCyNz nanotubes. The Raman spectroscopy shows that the as-grown BxCyNz nanotubes are radially phase separated into BN shells and carbon shells. The photoluminescence decay process is characterized by two time constants that are attributed to intra- and inter-BN sheet charge recombination, respectively. A comparison of the photoluminescence of BN nanotubes to that of hexagonal BN is consistent with the existence of a spatially indirect band gap in multiwalled BN nanotubes as predicted by theory.
Hexagonal boron nitride (h-BN) is isostructural with graphite and is the normal phase of BN that is stable at room temperature and ambient pressure. It is a wide band gap semiconductor with potential applications in optoelectronic devices. First principles local-density calculations have shown that the lowest band gap (4.07 eV) is indirect, located near the Brillouin-zone edges. However, because of the quasi-2D nature of the hexagonal structure, the lowest direct band gap is predicted to be close by at 4.2 eV.1 A wide range of lowest gap energies, such as 3.8,2 4.3,3 5.2,4 and 5.9 eV,5 have been reported by experimental studies using various techniques. When a hexagonal BN sheet is rolled up into a singlewalled BN nanotube (NT), its electronic structure is very different from that of carbon nanotubes because of the wide gap of BN sheets as opposed to the zero gap in graphite. In contrast to carbon nanotubes, which have diverse electronic properties depending on their structure, the band gaps of BN NTs are predicted theoretically to be approximately equal to that of h-BN, nearly independent of their radius and chirality, except for a band gap narrowing in thin NTs (diameter < ∼0.8 nm) as a result of sp3 (π) hybridization * Corresponding author. E-mail: [email protected]
. † Materials Sciences Division, Lawrence Berkeley National Laboratory. ‡ Department of Physics, University of California. § Molecular Foundry, Lawrence Berkeley National Laboratory. | Department of Materials Science and Engineering, University of California. 10.1021/nl049862e CCC: $27.50 Published on Web 03/18/2004
© 2004 American Chemical Society
induced by the high curvature.6 In this context, the predicted structural independence of the electronic properties and thermal stability of BN NTs open promising opportunities for applications in nanoelectronic and nanophotonic devices. The optical properties of BN NTs are still not well understood because of poor sample quality and low lightemission efficiency. Recently, it was demonstrated that multiwalled BN and boron carbon nitride (BxCyNz) NTs can be synthesized in large quantities using a carbon nanotube-substituted reaction.7 Transmission electron microscopy (TEM) shows that highquality, nearly perfect layer-structured BN or BxCyNz NTs can be grown in either individual or bundled form. In this letter, we present the results of optical spectroscopy studies of such BN and BxCyNz NTs. Raman spectroscopy and continuous-wave and time-resolved photoluminescence have been carried out, and the results are compared to recent theoretical calculations. BxCyNz nanotubes were synthesized via the carbon nanotube-confined reaction using chemical vapor depositionderived carbon NTs together with B2O3 and N2 at 1600 °C for half an hour. Subsequent thermal oxidation treatment at 650 °C efficiently transformed the BxCyNz NTs into BN NTs. Details of sample synthesis and oxidation processes have been published elsewhere.7 The resulting product is a mixture of 60-70% multiwalled BxCyNz (or BN after oxidation) NTs and ∼30-40% BxCyNz (or BN) fullerene-like particles
Figure 2. Raman spectra of BN and BxCyNz nanotubes and bulk h-BN recorded at room temperature. Inset shows the main peak near 1366 cm-1.
Figure 1. TEM image of (a) BxCyNz nanotubes, (b) BN nanotubes, and (c) h-BN powder. Inset is the high-resolution TEM image.
(mostly), nanoparticles, and nanowires. Electron energy loss spectroscopy (EELS) shows that, prior to oxidation, the C/B atomic ratio is between 0.2 and 0.4 and that after oxidation it is reduced to ∼1500 ps. In Figure 4b, the two lifetimes obtained are plotted as a function of the emission energy. It can be seen that both lifetimes increase on the lower-energy shoulder of the PL peak. This is typical band-edge luminescence behavior in which the shorter lifetime of higher-energy carriers is attributed to the additional relaxation channel via thermalization to lower-energy states.15 The temporal behavior of the emission from the BxCyNz NTs is quantitatively similar to that of the BN NTs (not shown here). As a comparison, Figure 5 shows the lifetime plot of the h-BN sample. The plot shows qualitatively similar behavior but with several differences. Lifetime τ2 is longer in the BN 649
sheets and between different BN shells/sheets, respectively. As the h-BN sheets form multiwalled NTs, τ1 is reduced because point defects induced on BN shells act as additional recombination centers. Lifetime τ2 is increased as a result of the spatial separation of electrons and holes. In both the BN NT and the h-BN samples, the intensity of the τ1-related emission is larger by a factor of 5-10 than the τ2-related emission. This indicates that the charge relaxation and recombination processes are predominantly occurring within individual hexagonal BN shells in the multiwalled NT structure. This behavior is consistent with the recent observation of strongly delocalized π plasmons along the tube axis in multiwalled BN NTs as studied by EELS.16 In summary, we have observed the strong photoluminescence of multiwalled BN and BxCyNz nanotubes at room temperature. A temporal analysis of the PL signals reveals a charge recombination process dominated by the fast recombination occurring within individual BN sheets. The slower decay process is attributed to the charge transfer and recombination across different BN sheets and shows behavior that is consistent with the predicted spatially indirect band gap of multiwalled BN NTs. Results of Raman spectroscopy confirm that the multiwalled BxCyNz NTs are structured into radially phase-separated BN and carbon shells. Figure 4. (a) Time-resolved photoluminescence of BN NTs. The wavelength window for each curve is 5 nm. The solid curves show the best fit using a double-exponential function. (b) Lifetimes obtained from the fitting with the double-exponential decay function.
Acknowledgment. This work is supported by the Director, Office of Science, Office of Basic Energy Sciences, Division of Materials Sciences and Engineering of the U.S. Department of Energy under contract no. DE-AC0376SF00098. W.-Q. H . and A.Z. acknowledge support from the Molecular Foundry, LBNL. References
Figure 5. Lifetimes of h-BN obtained from fitting with the doubleexponential function.
NTs than in the h-BN sample by more than 50% in the main peak region. This effect is tentatively attributed to the spatially indirect nature of the band gap in the multiwalled BN NTs. Similar to type-II offset planar quantum wells, the recombination probability of electrons and holes is reduced as a result of the spatial separation of their wave function, which increases the lifetime of the PL. However, lifetime τ1 is shorter (by 40%) in the BN NTs. Therefore, we can speculate that the decay processes associated with lifetimes τ1 and τ2 involve recombination within single BN shells/ 650
(1) Xu Y.; Ching, W. Y. Phys. ReV. B 1991, 44, 7787-7798. (2) Rand M. J.; Roberts, J. F. J. Electrochem. Soc. 1968, 115, 423427. (3) Zupan J.; Kolar, D. J. Phys. C 1972, 5, 3097-3100. (4) Hoffman, D.; Doll G. L.; Eklund, P. C. Phys. ReV. B 1984, 30, 60516056. (5) Tarrio C.; Schnatterly, S. E. Phys. ReV. B 1989, 40, 7852-7859. (6) Rubio, A.; Corkill, J. L.; Cohen, M. L. Phys. ReV. B 1994, 49, 50815084. Blase, X.; Rubio, A.; Louie, S. G.; Cohen, M. L. Europhys. Lett. 1994, 28, 335-340. (7) Han, W. Q.; Mickelson, W.; Cumings, J.; Zettl, A. Appl. Phys. Lett. 2002, 81, 1110-1112. (8) Suenaga, K.; Collix, C.; Demoncy, N.; Loiseau, A.; Pascard, H.; Willaime, F. Science 1997, 278, 653-655. (9) Popov, V. N. Phys. ReV. B 2003, 67, 085408. (10) Nemanich, R. J.; Solin, S. A.; Martin, R. M. Phys. ReV. B 1981, 23, 6348-6356. (11) Rao, A. M.; Richter, E.; Bandow, S.; Chase, B.; Eklund, P. C.; Williams, K. A.; Fang, S.; Subbaswamy, K. R.; Menon, M.; Thess, A.; Smalley, R. E.; Dresselhaus, G.; Dresselhaus, M. S. Science 1997, 275, 187-191. (12) Eklund, P. C.; Holden, J. M.; Jishi, R. A. Carbon 1995, 33, 959972. (13) de la Concha, R. A.; Wirtz, L.; Mevellec, J. Y.; Lefrant, S.; Rubio, A.; Loiseau, A. AIP Conf. Proc. 2003, 685, 384-388. (14) Okada, S.; Saito, S.; Oshiyama, A. Phys. ReV. B 2002, 65, 165410. (15) Kim, H. S.; Mair, R. A.; Li, J.; Lin, J. Y.; Jiang, H. X. Appl. Phys. Lett. 2000, 76, 1252-1254. (16) Fuentes, G. G.; Borowiak-Palen, E.; Pichler, T.; Liu, X.; Graff, A.; Behr, G.; Kalenczuk, R. J.; Knupfer, M.; Fink, J. Phys. ReV. B 2003, 67, 035429.
NL049862E Nano Lett., Vol. 4, No. 4, 2004